# X-ray Diffraction (XRD) - Philips Research

X-ray Diffraction (XRD) - Philips Research

X-ray Diffraction (XRD) - Philips Research

### You also want an ePaper? Increase the reach of your titles

YUMPU automatically turns print PDFs into web optimized ePapers that Google loves.

<strong>Philips</strong> <strong>Research</strong><br />

X-<strong>ray</strong>s are electromagnetic waves with a wavelength in the range of interatomic<br />

distances (0.1-10 Å).This match of length scales makes them suitable<br />

for the study of crystalline materials. For single-phase materials the<br />

crystal structure can be obtained directly using X-Ray diffraction (<strong>XRD</strong>).<br />

Materials Analysis<br />

With the help of a database of known structures <strong>XRD</strong> can be used for<br />

phase identification. Also crystal size, strain and preferred orientation of<br />

polycrystalline materials can be measured.The related technique of X-<strong>ray</strong><br />

reflection enables accurate determination of film thickness.<br />

X-<strong>ray</strong> <strong>Diffraction</strong> (<strong>XRD</strong>)<br />

• phase identification<br />

• texture or preferential orientation<br />

• crystallite size<br />

• residual stress<br />

• in-situ temperature and pressure studies<br />

• high resolution diffraction<br />

• layer thickness measurements

Principles<br />

When X-<strong>ray</strong> radiation is directed on a sample,<br />

the X-<strong>ray</strong>s are scattered (“diffracted”) by<br />

electrons present in the material. If the atoms<br />

in the material are arranged in a regular structure,<br />

i.e. if the material is crystalline, this scattering<br />

results in maxima and minima in the diffracted<br />

intensity. The signal maxima follow<br />

Bragg’s law nλ = 2dsinΘ. Here n is an integer,<br />

λ is the X-<strong>ray</strong> wavelength, d is the distance<br />

between crystal lattice planes and Θ is the diffraction<br />

angle (see fig. 1).Thus, for each lattice<br />

spacing d, Bragg’s law predicts a maximum at a<br />

characteristic diffraction angle Θ. During an<br />

X-<strong>ray</strong> diffraction (<strong>XRD</strong>) measurement the<br />

angles of incidence and detection are scanned.<br />

When the intensity of detected X-<strong>ray</strong>s is plotted<br />

as a function of angle Θ an X-<strong>ray</strong> diffraction<br />

pattern is obtained, which is characteristic<br />

for the sample material.<br />

The usual information depth of <strong>XRD</strong> measurements<br />

ranges from a few micrometers to a<br />

few hundred micrometers, depending on the<br />

density of the material. By using a very small,<br />

fixed incidence angle of the X-<strong>ray</strong>s (so-called<br />

grazing incidence measurement) also thin layers<br />

of only a few nanometers can be investigated.<br />

Source<br />

d<br />

θ<br />

Fig. 1: Schematic representation of diffraction of<br />

X-<strong>ray</strong>s in a crystalline material. Bragg’s law is<br />

satisfied when the pathlength difference of the<br />

X-<strong>ray</strong>s (indicated in green) is equal to nλ. The<br />

diffraction angle Θ is half the angle between the<br />

incident and diffracted X-<strong>ray</strong>s.<br />

Detector<br />

θ<br />

Techniques and applications<br />

Phase Identification<br />

In an X-<strong>ray</strong> diffraction pattern the position<br />

and intensity of the maxima are characteristic<br />

for the crystallographic structure and the<br />

atomic composition of the material. In case of<br />

a multi-phase composition, the resulting pattern<br />

is a combination of the patterns of all<br />

structures present. Phase identification can be<br />

done by matching the <strong>XRD</strong> pattern with reference<br />

patterns of pure substances.<br />

Fig. 2 shows an example of an <strong>XRD</strong> pattern of<br />

a temperature-resistant material used in the<br />

construction of a high temperature furnace. In<br />

this particular case the reaction between the<br />

furnace wall and the furnace content has been<br />

studied.The <strong>XRD</strong> pattern (dark green) can be<br />

matched with a mixture of the crystallographic<br />

structures of mullite (red bars), corundum<br />

(green bars) and baddeleyite (purple bars).<br />

Each colored bar of a reference pattern corresponds<br />

to a characteristic interatomic spacing<br />

(d) of the crystallographic structure.<br />

Quantitative information on single phase and<br />

multi-phase materials can be obtained using<br />

pattern calculation and pattern fitting methods<br />

intensity (a.u.)<br />

Mullite Al 6 Si 2 O 13<br />

Corundum Al 2 O 3<br />

25 30 35 40<br />

15 20<br />

Baddeleyite ZrO 2<br />

2θ angle (°)<br />

Fig. 2: <strong>XRD</strong> pattern of furnace material and<br />

reference patterns of identified components.<br />

(so-called Rietveld refinement). In combination<br />

with the use of standard materials this<br />

approach can supply accurate values for sample<br />

composition, crystal symmetry, unit-cell<br />

dimensions, atom positions, site-occupancy<br />

factors, etc.

intensity (a.u.)<br />

Preferential Orientation, Texture<br />

In powder samples the number of crystalline<br />

grains (“crystallites”) is large. Their orientation<br />

is usually random. However, preferential<br />

orientation of the crystallites can occur. In<br />

such a case the sample is called “textured”.<br />

Especially in thin films and rolled metal sheets,<br />

texture can be found.The presence of preferential<br />

orientation is already visible in a standard<br />

diffraction pattern. This is illustrated in<br />

fig. 3, where two diffraction patterns of crystalline<br />

MgO are shown. Although the MgO<br />

crystal structure is identical in both samples,<br />

the orientation distribution is different. This<br />

difference manifests itself in the relative intensities<br />

of the diffraction peaks. The pattern of<br />

an MgO powder (purple curve) represents a<br />

sample with randomly oriented crystals,<br />

whereas the pattern of the oriented thin MgO<br />

layer on a glass substrate (red curve) displays<br />

a textured polycrystalline layer.<br />

The accurate description of the texture present<br />

can be determined by measuring diffraction<br />

in three dimensions. By rotating and tilting<br />

the sample with respect to the X-<strong>ray</strong> beam<br />

an orientation distribution of the crystallites<br />

can be calculated.<br />

Crystallite size, micro-strain and residual<br />

stress determinations<br />

<strong>XRD</strong> can also supply information about deformation<br />

of a crystalline sample. Deformation<br />

(also referred to as strain) of a crystal lattice<br />

will result in a change in the inter-atomic distances.<br />

The effect on a diffraction pattern<br />

depends on whether the deformation occurs<br />

on a local (microscopic) or on a global (macroscopic)<br />

scale. Microscopic deformation, i.e. local<br />

variation of the interatomic distances in a sample,<br />

is referred to as micro-strain. In this case,<br />

<strong>XRD</strong> analysis of an entire sample will display a<br />

range of deviations from the expected interatomic<br />

distances (d).This leads to peak broadening.<br />

The width of a diffraction peak is also<br />

influenced by the crystallite size: a large crystallite<br />

size causes sharp reflections, whereas a<br />

small size leads to broad reflections. Although<br />

size and strain both result in peak broadening,<br />

their effects can be separated since their angular<br />

dependence is different. The effect crystal<br />

size can have on an <strong>XRD</strong> pattern is shown in<br />

fig. 4.<br />

35 40 45<br />

62.5 63.0 63.5<br />

MgO powder<br />

MgO thin film<br />

Fig. 3: <strong>XRD</strong> patterns of a thin MgO film with a<br />

preferential orientation and of randomly oriented<br />

polycrystalline MgO powder.<br />

Fig. 4: <strong>XRD</strong> peak profiles of polycrystalline silver<br />

with different crystallite sizes.<br />

intensity (a.u.)<br />

material.The deviation in the peak position can<br />

be translated into macroscopic strain and into<br />

a residual stress if mechanical material constants<br />

are known.<br />

Non-ambient and in-situ <strong>XRD</strong><br />

For <strong>XRD</strong> studies under non-ambient conditions<br />

(gas pressures up to 60 bar and/or temperatures<br />

up to 1600°C) a special vessel can<br />

be attached to an instrument. This allows the<br />

study of phase transformations induced by<br />

temperature, crystallization, and/or incorporation<br />

of interstitial atoms in a material, e.g.<br />

hydrogen absorption.<br />

For qualitative analysis of materials with relatively<br />

large lattice spacings, e.g. polymers and<br />

liquid crystals, and for studying changes in<br />

such materials a special X-Ray detector and a<br />

sample heater are available. The two-dimensional<br />

nature of the detector permits the<br />

50 55 60 65 70 75 80<br />

2θ angle (°)<br />

> 1000 Å<br />

600 Å<br />

100 Å<br />

64.0 64.5 65.0 65.5 66.0 66.5 67.0<br />

2θ angle (°)<br />

rapid collection of diffracted and scattered X-<br />

<strong>ray</strong>s and provides this way the unique capability<br />

of directly imaging phase transformations<br />

and orientation changes in a diffraction pattern.<br />

An example is given in fig. 5, which shows<br />

2-D patterns of a liquid crystalline material. In<br />

the pattern recorded at 200°C a broad diffuse<br />

ring can be seen, indicating that the material<br />

has no crystalline structure, i.e. it is a liquid.<br />

The pattern recorded at room temperature<br />

shows discrete rings, which means that the<br />

material is crystalline.The intensity differences<br />

that are visible along some of the rings indicate<br />

that the crystallites have certain preferred<br />

orientations.<br />

Fig.5: 2-D diffraction images of a liquid crystalline<br />

material recorded at room temperature (left) and<br />

at 200°C (right).<br />

Deformation on a macroscopic scale, i.e. more<br />

or less homogeneous in a sample, causes diffraction<br />

peak shifts. These shifts reflect the<br />

change in interatomic distances in the

Intensity (a.u.)<br />

layer thickness<br />

fringes<br />

layer peak<br />

SiGe(C)<br />

substrate peak<br />

Si 0.8 Ge 0.2<br />

Si 0.8 Ge 0.2 C 0.004<br />

<strong>Philips</strong> <strong>Research</strong> Materials Analysis<br />

offers a full range of analytical methods and<br />

expertise to support both research and<br />

manufacturing, serving customers by taking an<br />

integral, solution-oriented approach.<br />

making the invisible visible<br />

67 68<br />

Fig. 6: High resolution measurement of Si 0.8 Ge 0.2<br />

and Si 0.8 Ge 0.2 C 0.004 layers on Si-wafers.<br />

Fig. 7: Layer thickness determination of a single<br />

and double layer-stack.<br />

69 70 71<br />

2θ angle (°)<br />

For more information:<br />

Tel./fax: +31 -40-27 43210/43075<br />

E-mail: materialsanalysis@philips.com<br />

http://www.philips.com/materialsanalysis<br />

http://pww.natlab.research.philips.com:25222/<br />

Technical Note 13<br />

October 2004<br />

Peter Graat<br />

67 nm metal layer<br />

21 nm Si 3 N 4 + 18 nm metal layer<br />

Intensity (a.u.)<br />

0 1<br />

2 3 4<br />

2θ angle (°)<br />

High Resolution X-<strong>ray</strong> diffraction<br />

Thin layers are often grown epitaxially on a<br />

crystalline substrate. Epitaxy implies a perfect<br />

match between the crystal lattices of the substrate<br />

and the crystalline layer that is grown<br />

on top of it. With an extremely well defined<br />

X-<strong>ray</strong> beam it is possible to measure minor<br />

changes in the degree of epitaxiality of the<br />

thin layer or the crystal quality.The thickness<br />

of thin layers and very small changes in crystal<br />

lattice dimensions resulting from differences<br />

in composition are also measurable.<br />

As an example, in fig. 6 high-resolution diffraction<br />

patterns of a SiGe layer and a SiGeC layer<br />

on top of a silicon substrate are displayed.<br />

Si x Ge y is a semiconductor material with superior<br />

electrical properties in comparison to<br />

pure silicon, but has the disadvantage of introducing<br />

strain and defects into the device.<br />

Si x Ge y C z is used to reduce this lattice mismatch<br />

between the thin layer and the substrate<br />

without significant loss of electrical<br />

properties. In fig. 6 the broad peak of the thin<br />

SiGe layer (blue curve) appears at a different<br />

angle (inter-atomic spacing) than the sharp<br />

peak from the silicon substrate.The peak shift<br />

observed is caused by the larger Ge-atoms<br />

incorporated in the silicon lattice leading to a<br />

larger lattice parameter. Due to the addition<br />

of carbon a peak shift to a larger angle (smaller<br />

lattice parameter) is seen in the red curve.<br />

The smaller difference in lattice parameter<br />

between the substrate and the thin layer<br />

reduces the strain in the thin layer.<br />

X-<strong>ray</strong> Reflectivity (XRR)<br />

X-<strong>ray</strong> reflectivity measurements are used to<br />

determine the thickness of thin layers and<br />

layer-stacks (3 to 300 nm) on a flat and<br />

smooth substrate. In the case of a single thin<br />

layer, reflection occurs at the surface of the<br />

thin layer and at the interface with the substrate.<br />

Interference of these two reflections<br />

results in a characteristic wave pattern of the<br />

reflected intensity as a function of the angle of<br />

incidence. In the case of a multi-layer, the<br />

reflected intensity is the result of the addition<br />

of the wave pattern of each layer. In fig. 7<br />

examples of such X-Ray reflectivity curves of<br />

a single and a double layer are shown. The<br />

absolute layer thickness is obtained from the<br />

difference in angular position of the visible<br />

fringes.<br />

Characteristics<br />

Sample type<br />

• solid substance as bulk (e.g. powders) or<br />

thin film (on a substrate)<br />

Sample size<br />

• few mm 2 to several cm 2 ;few mg<br />

for powders<br />

Resolution<br />

• spot dimensions typically 10*10 mm 2 , penetration<br />

depth ranging from 2 µm (Au) to<br />

120 µm (Al 2 O 3 )<br />

Detection limit<br />

• minority phases are detectable from<br />

approx. 1 wt% (phase identification),<br />

depending on the elements present<br />

• XRR: Layer thickness 3-300 nm, roughness<br />

up to 3 nm<br />

Advantages<br />

• fast technique<br />

• non-destructive<br />

• small sample amount required<br />

• in most cases no elaborate sample preparation<br />

necessary